1999 Reneker Fong Chun Beaded Nanofibers Formed During Electrospinning
Embed Size (px)
Transcript of 1999 Reneker Fong Chun Beaded Nanofibers Formed During Electrospinning
Beaded nanofibers formed during electrospinningH. Fong, I. Chun, D.H. Reneker*
Maurice Morton Institute of Polymer Science, The University of Akron, Akron, OH 44325-3909, USADedicated to Professor Ronald K. Eby on the occasion of his 70th birthday
Received 10 September 1998; received in revised form 6 October 1998; accepted 22 October 1998
Electrospinning is a straightforward method to produce polymer fibers from polymer solutions, with diameters in the range of 100 nm.Electrospun fibers often have beads in regular arrays. The viscoelasticity of the solution, charge density carried by the jet, and the surfacetension of the solution are the key factors that influence the formation of the beaded fibers. q 1999 Elsevier Science Ltd. All rights reserved.
Keywords: Electrospinning; Beaded nanofiber; Nanofiber
It was known in the early 1900s that if molten sealing waxwas electrified, solid fibers were ejected. Sealing wax isbrittle, and no viable commercial development of thisprocess for making fibers has resulted so far. Focus is nowon the liquid jets created by electric fields, the distortion ofliquid droplets in an electric field, the collapse of liquid jetsinto droplets, and the development of processes for electro-spraying paint and other liquids. In the past century, elec-trostatic spinning and related phenomena, such as aerosolspraying, atomization in the charged droplets and the forma-tion of particles, have received attention . Baumgarten, working at Dupont in the 1970s, published high speedphotographs and other data describing the formation offibers of an acrylic polymer by electrostatic spinning. Rene-ker  and co-workers characterized the electrospinningprocess and the physical properties of electrospun nanofi-bers.
Electrospun fibers often have beads as by products.The formation of beaded fibers has been observed widely. The electrospun beaded fibers are related to theinstability of the jet of polymer solution, which was studiedby Yarin  and Entov . They developed a mathema-tical model for the break-up of jets of polymer liquids,which did not include the effects of electric fields. In1962, Magarvey and Outhouse  found that the break-up of water jets depended on the electrical current. The more
current the water jet carried, the less likely it was to formdroplets. Huebner  also considered such electricalphenomena. Fang  electrospun beaded DNA nanofibers.Jaeger [15,16] reported beaded fibers spun from aqueoussolutions of poly(ethylene oxide) (PEO). He found thatthe bead diameter and spacing were related to the fiberdiameter: the thinner the fiber, the shorter the distancebetween the beads and the smaller the diameter of the beads.
Characterization of the formation of electrospun beadednanofibers shows that solution viscosity, net charge densitycarried by the electrospinning jet and surface tension of thesolution are the main factors. Higher viscosity favors forma-tion of fibers without beads, higher net charge density notonly favors formation of fibers without beads, but alsofavors the formation of thinner fibers. Surface tension drivestowards the formation of beads, hence reduced surfacetension favors the formation of fibers without beads.
Changing the polymer concentration can vary the solu-tion viscosity. The surface tension coefficient depends onthe polymer and solvent. For example, changing the ratio ofethanol to water can change the surface tension coefficientof the PEO solution. Net charge density carried by the jet inthe electrospinning process is primarily affected by theapplied electrostatic field and to a lesser extent by theconductivity of the solution. For example, the addition ofNaCl to a PEO/water solution is observed to increase the netcharge density carried by the spinning jet. The use of thequantity charge per unit volume (C/l) does not imply that thenet charge density is distributed uniformly throughout thejet. When the jet shape is changing rapidly, most of the netcharge is found to be near the surface. The net chargedensity on the jet can be reduced to a low value, by ions
Polymer 40 (1999) 45854592
0032-3861/99/$ - see front matter q 1999 Elsevier Science Ltd. All rights reserved.PII: S0032-3861(99)00068-3
* Corresponding author. Tel.: 1 1-330-972-6949; fax: 1 1-330-972-5290.
with polarity opposite to those carried by the jet, from acorona discharge in air.
An electrically driven jet of a low molecular weight liquidwill form droplets  (electrospraying). The formation ofthese droplets is due to the capillary breakup of the spinningjet by surface tension . For polymer solutions, thepattern of the capillary breakup is changed radically. Insteadof breaking rapidly, the filaments between the droplets arestabilized and a stable beads-on-string structure is formed.The reason for this is that the coiled macromolecules of thedissolved polymer are transformed by the elongational flowof the jet into oriented, entangled networks that persist as thefiber solidifies. The contraction of the radius of the jet,which is driven by surface tension, causes the remainingsolution to form beads.
As the viscosity of the solution is increased, the beadsbecome bigger, the average distance between beads longer,the fiber diameter larger, and the shape of the beads changesfrom spherical to spindle-like. As the net charge densityincreases, the beads become smaller and more spindle-like, while the diameter of fibers become smaller. Decreas-ing the surface tension make the beads disappear gradually.Neutralization of the charge carried by the jet favors theformation of beads, because the tension in the fiber dependson the net charge repulsion and the interaction of the netcharge with the electric field.
PEO, with an average weight molecular weight of 9 105
(g/mol), was obtained from Scientific Polymer ProductCompany and used without further purification. Distilledwater was used. The solutions were prepared at roomtemperature, and gently stirred to speed dissolution. ThePEO solution was held in a hemispherical metal spoon,which had an orifice of 0.3 mm diameter in its bowl. Thediameter of the spoon was about 2.0 cm and the thicknessabout 1.0 mm. The spoon was connected to a high-voltagesupply, which is capable of generating positive DC voltagesup to 30 kV. A flat piece of aluminum foil, placed 21.5 cmbelow the orifice, was used to collect the electrospun mate-rial. Currents were measured with a 100 mA meter attachedbetween the aluminum foil and ground. Neutralizing ionswere generated by using a negative 30 kV supply attached toa bundle of fine copper wires (d 0.4mm) to create a coronadischarge. The bundle of copper wires was put in a plastictube that was connected with an air blower. The airflow ratewas about 0.1 l/s. The outlet of the tube was 10 cm belowand 40 cm to the side of the metal spoon. The concentrationof the neutralizing ions was controlled by adjusting thenegative voltage between 0 and 18 kV.
The morphology of the electrospun nanofibers wasobserved with a Scanning Electron Microscope (ModelNo. JSM-5310) manufactured by Japan Electron OpticalLaboratory.
3. Results and discussion
Three series of solutions were prepared for the study: (1)PEO with distilled water only, (2) PEO and NaCl with
H. Fong et al. / Polymer 40 (1999) 458545924586
Table 1The preparation and characterization of the solutions
PEO (g) Water (g) Ethanol (g) NaCl (g) Solutionviscosity(centipoise)
1 1.00 100 13 77.8 3062 1.50 100 32 76.4 2953 2.00 100 74 76.0 2544 2.50 100 160 78.6 2345 3.00 100 289 77.6 2216 3.50 100 527 77.0 2127 4.00 100 1250 76.6 2048 4.50 100 1835 76.2 195
A 3.00 97 0.0015 375 76.2 83.4B 3.00 97 0.0060 392 74.8 47.4C 3.00 97 0.030 432 75.0 16.7D 3.00 97 0.150 431 76.0 3.61E 3.00 97 0.30 387 74.2 1.90F 3.00 97 1.50 362 76.4 0.462
I 3.00 97 0 402 75.8 110II 3.00 92 5 504 68.9 130III 3.00 87 10 623 63.1 180IV 3.00 77 20 889 59.3 269V 3.00 67 30 1129 54.7 333VI 3.00 57 40 1179 50.5 386
distilled water, and (3) PEO with distilled water and ethanol.The preparation and characterization of these solutions aresummarized in Table 1. The water used for samples 18 wasdistilled twice and the resistivity was 1629 V m. For othersamples, the water was distilled only once and the resistivitywas 165 V m. The resistivity increased as alcohol wasadded, because alcohol has a resistivity that is at least twoorders of magnitude greater than that of water.
To characterize the SEM images of the beaded nano-fibers shown in Figs. 14, the following measurementswere made: average bead length along the fiber axis(BL), average bead width perpendicular to the fiberaxis (BW), average fiber diameter (FD), average fiberlength between beads (FL), and the approximate ratio ofbead volume to fiber volume (AR). These are summarizedin Table 2.
H. Fong et al. / Polymer 40 (1999) 45854592 4587
1a: 13 centipoise 1b: 32 centipoise
1c: 74 centipoise 1d: 160 centipoise
1e: 289 centipoise 1f: 527centipoise
1g: 1250 centipoise 1h: 1835 centipoise
Fig. 1. The morphology of beaded fibers versus solution viscosity. Electric field is 0.7 kV/cm. The horizontal edge of each image is 20 microns long.
Fig. 1 shows the representative images of beads andbeaded fibers for solutions with a range of viscosity(samples 18). Beads and beaded fibers are less likely tobe formed for the more viscous solutions. The diameter ofthe beads become bigger and the average distance betweenbeads on the fibers longer as the viscosity increases. Mean-while, the shape